Presentation on theme: "Dr. Waseem Bahjat Mushtaha Specialized in prosthodontics"— Presentation transcript:
1 Dr. Waseem Bahjat Mushtaha Specialized in prosthodontics Dental CeramicsDr. Waseem Bahjat Mushtaha Specialized in prosthodontics
2 Imagine a restorative material, that can accurately duplicate tooth structure, such that an average person may find it difficult to distinguish between the two . Dental ceramics holds such a promise. One might argue that composite resins have a similar esthetic potential. However, there is a big difference-dental ceramics are certainly far more durable. They are far more stronger, wear resistant, and virtually indestructible in the oral environment. They are impervious to oral fluids and absolutely biocompatible. They do have some drawbacks which will be discussed subsequently. Because of their huge potential, it is still a fast growing area in terms of research and development.
3 USES AND APPLICATIONS 1-Inlays and onlays 2- Esthetic laminates (veneers) over natural teeth3- Single (all ceramic) crowns4- Short span (all ceramic) bridges5- As veneer for cast metal crowns and bridges (metal ceramics)6- Artificial denture teeth (for complete denture and partial denture use)7- Ceramic orthodontic brackets
4 CLASSIFICATION OF DENTAL PORCELAINS According to Firing Temperature1-High fusing 1300°(for denture teeth)2-Medium fusing 1101 to 1300°(for denture teeth)3- Low fusing 850 to 1100°(for crown and bridge use)4-Ultra low fusing less than 850 (used with titanium)
5 According to Type1-Feldspathic or conventional porcelain2-Aluminous porcelain3- Leucite reinforced4-porcelain Glass infiltrated alumina5- Glass infiltrated spinell6- Glass ceramic
6 According to Use1-Porcelain for artifical denture teeth2- Jacket crown, veneer and inlay porcelain3-Metal ceramics4- Anterior bridge porcelain.According to Processing Method1-Sintered porcelain2- Cast porcelain3- Machined porcelain.
7 BASIC CONSTITUENTS AND MANUFACTURE Because of the wide variety of porcelain products available in the market, it is virtually impossible to provide a single composition for them all. Traditionally, porcelains were manufactured from a mineral called feldspar. These porcelains are referred to as feldspathic porcelains. As porcelain technology improved other specialized porcelains were introduced, like reinforced core porcelains, opaquer porcelains, glass ceramics, glazes, etc. Obviously their composition would certainly differ from the traditional feldspathic porcelains. Our discussion will center around feldspathic porcelain.
8 Basic StructureBasically porcelain is a type of glass. Therefore its basic structure is similar to that of glass. The basic structure therefore consists of a three dimensional network of silica (silica tetrahedra). Pure glass melts at too high a temperature for dental use. Adding certain chemicals lowers the melting temperature by disrupting the silica network. The glass obtains porcelain like qualities when the silica network is broken by alkalies like sodium and potassium. This also lowers the fusion temperature. These chemicals are therefore known as glass modifiers or fluxes. Other substances which act like glass modifiers are alumina (Al,03) and boric oxide (B,03)· Boric oxide forms its own separate network in between the silica network. Adding certain opacifiers reduces the transparency and completes the transformation to dental porcelain.
10 FeldsparIt is a naturally occurring mineral and forms the basic constituent of feldspathic porcelains. Most of the components needed to make dental porcelain are found in feldspar. It thus contains potash (K20), soda (Na20), alumina (AI203) and silica (Si02). It is the basic glass former. When fused at high temperatures (during manufacture) it forms a feldspathic glass containing potash feldspar (K,O.Al203.6SiO,) or soda feldspar (Na20.A1203.6SiO,). Pure feldspathic glass is quite colorless and transparent. As explained earlier, various glass modifiers and opacifiers are added to alter its sintering temperature, viscosity, thermal coefficient of expansion (CTE) and appearance.
11 KaolinIt is a white clay like material (hydrated aluminum silicate). It gives porcelain its properties of opaqueness when mixed with water, it gives consistency to the mix and forms a workable mass of porcelain during molding and when subjected to high temperatures, it binds the particles and maintains the framework . Some manufacturers use sugar or starch instead of kaolin.QuartzQuartz is a form of silica. Ground quartz acts as a refractory skeleton, providing strength and hardness to porcelain during firing. It remains relatively unchanged during and after firing.
12 AluminaAluminum oxide (alumina) replaces some of the silica in the glass network. It gives strength and opacity to the porcelain. It increases the viscosity of porcelain during firing.Glass ModifiersAlkalies such as sodium, potassium and calcium are called glass modifiers. Glass modifiers lower the fusion temperature and increase the flow of porcelain during firing. They also increase the CTE (important in metal ceramics). However, too high a concentration of glass modifiers is not good for the ceramic because: It reduces the chemical durability of the ceramic. It may cause the glass to devitrify (crystallize) Another glass modifier is boric oxide (H203). It forms its own glass network (also called lattice) interspersed between the silica network (lattice).
13 OpacifiersSince pure feldspathic porcelain is quite colorless, opacifiers are added to increase its opacity in order to simulate natural teeth. Oxides of zirconium, titanium and tin are commonly used opacifiers.Color ModifiersNatural teeth come in a variety of shades. In addition, it acquires external stains from the environment. Thus color modifiers are required to adjust the shades of the dental ceramic. Various metallic oxides provide a variety of color, e.g. titanium oxide (yellowish brown), nickel oxide (brown), copper oxide (green), manganese oxide (lavender), cobalt oxide (blue), etc. They are fused together with regular feldspar and then reground and blended to produce a variety of colors.
14 Other Specialized Porcelain Powders Glazes It is a special type of colorless porcelain applied to the surface of the completed ceramic restoration to give it a glossy lifelike finish . Obviously they do not contain opacifiers. They must have a lower fusion temperature and therefore must contain a lot of glass modifiers. This also makes them somewhat less chemically durable.StainsThey are porcelain powders containing a high concentration of color modifiers (as described previously). They too have a lower fusion temperature made possible by an increased content of glass modifiers. Stains are used to provide individual color variation in the finished restoration
15 Opaquer PorcelainsIt is a specialized type of porcelain which is used to conceal the metal core in PFM (metal ceramic) restorations . It is the first layer applied before the addition of the regular porcelain. Obviously it contains a high concentration of opacifiers, Some amount of color modifiers are also added
16 Reinforced Core Porcelains These are specialized porcelains containing a high concentration of a reinforcing material. The reinforced porcelains are stronger than regular feldspathic porcelains. They are used to create a strong inner core which imparts strength to the ceramic. A variety of reinforcing materials are currently being used. They include:1-Alumina (alumina reinforced porcelain)2-MgAl20, (spinell)3- Leucite (leucite reinforced porcelain).ManufactureTraditionally, porcelain powders are manufactured by a process called fritting. Various components are mixed together and fused. While it is still hot, it is quenched in water. This causes the mass to crack and fracture, making it easier to powder it. The frit is ground to a fine powder and supplied to the consumer in bottles. Most of the chemical reaction takes place during the manufacture (pyrochemical reaction). During subsequent firing in the dental laboratory, there is not much of chemical reaction). The porcelain powder simply fuses together to form the desired restoration.
17 PARTS OF A CERAMIC RESTORATION Currently, there are so many ceramic systems which can be quite confusing to the dental student. For simplicity of explanation we can divide the ceramic restoration into 2 parts1- Core (or substructure)2- VeneerCore The core should be strong as it provides support and strength for the crown. Manufacturers have concentrated on strengthening the core through various means. The stronger the core, the stronger the crown. The core also functions as the matrix. The matrix is a supporting frame. Freshly mixed porcelain is like wet sand. It needs to be supported while it is being condensed and built up. The freshly built unfired porcelain is very weak and fragile. Without the support of a matrix it would certainly breakup and collapse. The core is therefore usually constructed first. The rest of the restoration is built up on this core. The cores or substructures are of two basic types depending on whether it is an all porcelain crown or a metal ceramic crown.1-Metal core Porcelain or2- ceramic core
18 VeneerThe core is usually anesthetic. The esthetics is improved by additional layers of ceramic known as veneer porcelains. The core is veneered with various types of ceramic powders like dentin, enamel, cervical and transparent. It can also be surface stained and finally glazed.
19 CLASSIFICATION AND DESCRIPTION OF CERAMIC SYSTEMS The ceramic restorations available today may be metal bonded or made completely of ceramic. Based on the substructure or core material used we have two basic groups. They are further divided based on the fabrication method.A-Metal-ceramic (metal bonded or PFM) restorations1-Cast metal ceramic restorationsCast noble metal alloys- Cast base metal alloys- Cast titanium (ultra low fusing porcelain)2- Swaged metal ceramic restorations- Gold alloy foil coping (Renaissance, Captek)- Bonded platinum foil copingB- All ceramic restorations1. Platinum foil matrix constructed porcelains- Conventional porcelain jacket crown-Porcelain jacket crown with aluminous core- Ceramic jacket crown with leucite reinforced core (Optec HSP)
21 METAL CERAMIC RESTORATIONS Synonyms Porcelain fused to metal or PFM, metal bonded restorations. The first porcelain jacket crowns (PJC) of a century ago did not have a strengthening core and were therefore very weak. Later in 1965, Mclean developed the aluminous core porcelains. The alumina reinforced core made the ceramic crown stronger by interrupting crack propagation. At around the same time, the metalceramic system was developed. The cast metal core (called coping) strengthened the porcelain restoration immensely and soon it became the most widely used ceramic restoration. According to a 1994 survey, 90 percent of all ceramic restorations are porcelain fused to metal. The metal ceramic system was possible because of some important developments.1-Development of a metal and porcelain that could bond to each other2-Raising of the CTE of the ceramic in order to make it more compatible to that of the metal.This obviously meant that a lot of research had to go into both porcelain and metal composition before they could be used for metal ceramics.
22 CAST METAL CERAMIC RESTORATIONS This is one of the most commonest ways of constructing a ceramic restoration. Because of the strong metal frame it is possible to make long span bridges. It can also be used in difficult situations where an all ceramic restoration cannot be given because of high stresses and reduced preparation depth.Uses1- Single anterior and posterior crowns2- Short and long span anterior and posterior bridges
23 Composition of Ceramic for Metal Bonding Feldspathic porcelains are used for metal bonding. The basic composition is quite similar except for the higher alkali content (soda and potash). The higher alkali content was necessary in order to raise the CTE. Unfortunately this also increased the tendency of the ceramic to devitrify and appear cloudy A special opaquer powder is needed to mask the underlying metal so that it does not show through the ceramic . The opaquer powder has a high content of opacifiers. Similarly, the composition of glazes would be different. Glazes have a higher concentration of glass modifiers like soda, potash and boric oxide.
24 Supplied asOne typical kit consists of1- Enamel porcelain powders in various shades (in bottles)2-Dentin porcelain powders in various shades (in bottles)3- Liquid for mixing enamel, dentin, gingival and transparent4- Opaquer powders in various shades/ together with a liquid for mixing5- Gingival porcelain powder in various shades6-Transparent porcelain powder7- A variety of stain (colon) powders8- Glaze powder9- Special liquid for mixing stains and glaze.
25 MANIPULATION AND TECHNICAL CONSIDERATIONS Construction of the Cast Metal Coping or FrameworkA wax pattern of the intended restoration is constructed and cast in metal. A variety of metals are used for the frame, like noble metal alloys, base metal alloys and recently titanium
26 Metal PreparationA clean metal surface is essential for good bonding. Oil and other impurities form the fingers can contaminate. The surface is finished with ceramic bonded stones or sintered diamonds. Final texturing is done by sandblasting with an alumina air abrasive, which aids in the bonding. Finally, it is cleaned ultrasonically, washed and dried.Degassing and OxidizingThe casting (gold porcelain systems) is heated to a high temperature (980°C) to burn off the impurities and to form an oxide layer which help in the bonding. Degassing is done in the porcelain furnace.OpaquerThe opaquer is a dense yellowish white powder supplied along with a special liquid. It is used to cover the metal frame and prevent it from being visible. The metal framework is held with a pair of locking forceps. Opaquer powder is dispensed on to a ceramic palette and mixed with the special liquid to apaste like consistency . It is carried and applied on to the metal frame with a brush and condensed . The excess liquid is blotted with a tissue. The opaquer is built up to a thickness of 0.2 mm. The casting with the opaquer is placed in a porcelain furnace and fired at the appropriate temperature . Opaquer may be completed in two steps.
27 CondensationThe process of packing the powder particles together and removing the excess water is known as condensation.PurposeProper condensation packs the particles together. This helps minimize the porosity and reduce the firing shrinkage. It also helps to remove the excess water.Condensation TechniquesVibrationMild vibration by tapping or running a serrated instrument on the forceps holding the metal frame by helps to pack the particles together and bring out the excess water. An ultrasonic vibrator is also available for this purpose.SpatulationA small spatula is used to apply and smoothen the wet porcelain. This action helps to bring out the excess water.Dry powderDry powder is placed on the side opposite a wet increment. The water moves towards the dry powder pulling the wet particles together.
28 Dentin and EnamelThe dentin powder (pink powder) is mixed with distilled water or the liquid supplied. A glass spatula should be used (ceramic powder is abrasive and can abrade the metal and contaminate the porcelain). The bulk of the tooth is built up with dentin. A portion of the dentin in the incisal area is cut back and enamel porcelain (white powder) can be added . After the build-up and condensation is over, it is returned to the furnace for sintering.AdditionsIt is not necessary to build up the restoration in one step. Large or difficult restoration may be built up and fired in 2 or 3 stages. After each firing the porcelain may be shaped by grinding and additional porcelain is placed in deficient areas. Each additional firing is done at a lower temperature. Caution One must not subject the restoration to too many firings. Too many firings can give rise to a over translucent, lifeless restoration.Gingival and Transparent PorcelainThe enamel of some natural teeth may appear transparent. This is usually seen near the incisal edges. If present it can be duplicated using transparent porcelain. The cervical portions of natural teeth may appear more darker (e.g. more yellow) than the rest of the tooth. When indicated cervical porcelains are used to duplicate this effect (They are also referred to as gingival or neck dentin).
29 Surface Staining, Characterization and Effects Natural teeth come in variety of hues and colors. Some of them are present at the time of eruption (intrinsic, e.g. white fluorosis stains), while others are acquired over a period of time from the environment (extrinsic, e.g. cervical stains). Staining and characterization helps make the restoration look natural and helps it to blend in with the adjacent teeth . The stain powders are mixed with a special liquid, applied and blended with a brush. With more and more emphasis on recreating the natural look, effects are created using special techniques. This includes defects, cracks or other anomalies within the enamel.GlazingBefore final glazing, the restoration is tried in the mouth by the dentist. The occlusion is checked and adjusted by grinding. Final alterations can be made to the shape of the restoration by the dentist. The restoration is now ready for the final step which is the glazing. The restoration is smoothed with a stone prior to glazing. Glazing is the process by which the restoration is given a smooth glossy surface
30 Objectives of glazing1- Glazing enhances esthetics2- Enhances hygiene3- Improves the strength. Glazed porcelain is much stronger that unglazed ceramic. The glaze inhibits crack propagation.4-Reduces the wear of opposing teeth. Unglazed porcelain can accelerate wear of the opposing natural teeth
31 Type1- Over glazeThe glaze powder is mixed with the special liquid and applied on to the restoration. The firing temperature is lower than that of the body porcelain. The firing cycle does not usually include a vacuum. Chemical durability of over glazes is lower because of the high flux content.2- Self glazeA separate glaze layer is not applied. Instead the restoration is subject to a controlled heating at its fusion temperature. This causes only the surface layer to melt and flow to form a vitreous layer resembling glaze.Glazing versus Conventional PolishingPorcelain can be polished using conventional abrasives. Porcelain is an extremely hard material and is quite difficult to polish. However, glazing is still superior to conventional polishing.
32 FiringThe process of sintering and fusing the particles of the condensed mass is known as firing. The powder particles flow and fuse together during firing. Making the restoration dense and strong. Firing is done in a porcelain furnace.The Porcelain FurnaceFiring is carried out in a porcelain furnace . There are many companies which manufacture furnaces. Modem furnaces are computer controlled and have built in programs to control the firing cycle. The programs can also be changed by the operator.Firing CycleThe entire program of preheating, firing, subjecting to vacuum, subjecting to increased pressure, holding and cooling is known as a firing cycle. The firing cycles vary depending on the stage- opaquer firing, dentin firing, glaze firing, etc. The firing temperature is lowered gradually for each subsequent firing cycle. The opaquer has the highest temperature and the glaze has the lowest.PreheatingThe condensed mass should not be placed directly into the hot furnace. This can cause a rapid formation of steam which can break up the mass. Modern furnaces have a mechanism whereby the work is gradually raised into the furnace. This is known as preheating.Vacuum FiringDuring firing of the porcelain, a vacuum (negative pressure) is created in the furnace. This helps to reduce the porosity in the ceramic. The vacuum is later released raising the pressure in the furnace. The increased pressure helps to further reduce the size of any residual air bubbles not eliminated by the vacuum. The vacuum is not activated during the glaze firing.CoolingThe cooling of the fired porcelain should be well controlled. Rapid cooling can cause the porcelain to crack or it can induce stresses inside which weaken the porcelain. Cooling is done slowly and uniformly and is usually computer controlled.
33 PORCELAIN-METAL BONDFalls into two groups:-Chemical bonding across the porcelain-metal interface.- Mechanical interlocking between porcelain and metal.Chemical BondingCurrently regarded as the primary bonding mechanism. An adherent oxide layer is essential for good bonding. In base metals chromic oxide is responsible for the bond. In noble metal alloys tin oxide and possibly iridium oxide does this role. Ocassionally one does come across a metal-ceramic restoration which has failed because of poor metal-ceramic bonding
34 Mechanical Interlocking In some systems mechanical interlocking provides the principal bond. Presence of surface roughness on the metal oxide surface gives retention, especially if undercuts are present, wettability is important for bonding.Advantages of Cast Metal Ceramic Restorations1- Better fracture resistance because of the metal reinforcement.2- Better marginal fit because of the metal frame.Disadvantages1-Comparatively less esthetic (when compared to the all porcelain crown) because of the reduced translucency as a result of the underlying metal and the opaquer used to cover it.2- Margins may appear dark because of the metal. This sometimes shows through the gingiva causing it to appear dark and unesthetic.
35 OTHER METAL CERAMIC SYSTEMS Swaged Gold Alloy Foil-Ceramic Crowns Gold alloy foils (Renaissance and Captek) are a novel way of using metal without having to cast it. They come in a fluted form and is adapted to the die by swaging and burnishing. The foil coping is carefully removed and then flame sintered (fused). An interfacial alloy powder is applied and fired (it helps to bond the ceramic to the metal). Porcelain is then condensed and fired to form a crown.Advantages .1- The thinner foil alloy coping allows a greater thickness of ceramic thereby improving the esthetics.2- The underlying alloy is gold colored which gives more warmth and life to the restoration.Bonded Platinum Foil-Ceramic CrownsA platinum foil coping is constructed on the die. To improve the bonding of the ceramic to the platinum foil coping, an electrodeposition technique is used. The advantages of using bonded platinum foil is similar to that for swaged gold alloy foil.
36 The Electrodeposition Technique This is a technique used to improve both esthetics and bonding. A layer of pure gold is electrode posited onto the metal. This is quickly followed by a quick minimal deposition of tin over the gold.The advantages are1-The gold color enhances the vitality ofthe porcelain, thereby enhancing esthetics (the normal technique requires a heavy unesthetic opaque layer to cover the dark metal oxide surface). The tin helps in chemical bonding (through formation of tin oxide).2- Improved wetting at the gold-porcelain interface thereby reducing porosity.The electrodeposition technique can be used on metals such as stainless steel, cobalt chromium, titanium and other non-gold and low gold alloys
37 THE ALL CERAMIC RESTORATIONS The all ceramic restoration is a restoration without a metallic core or substructure. This makes them esthetically superior to the metal ceramic restoration. Unfortunately they are not as strong. For a long time metal ceramics continued to be the restoration of choice. In the meantime, research continued on strengthening the ceramic core as manufacturers concluded that the all ceramic restoration would be esthetically superior to the metal ceramic restorations. Current developments have yielded stronger core porcelains. Ceramics have come a long way from the days when all porcelain was attempted only for single anterior crowns. Manufacturers today claim the new generation ceramics are capable of producing not only single crowns but anterior and even posterior all ceramic bridges as well.
38 The all ceramic restorations may be described under the following: 1- Porcelain jacket crowns-Porcelain jacket crown (traditional)Porcelain jacket crown with aluminous core2- Ceramic jacket crown with leucite reinforced core (Dicor)3-Injection moulded (leucite reinforced) glass ceramic jacket crown (IPS Empress)4- Ceramic restoration with glass infiltrated aluminous core (Incerarn)5- Ceramic restoration with glass infiltrated spinell core (lnceram spinell)6-Ceramic restoration with glass infiltrated spinell core (lnceram spinell)7-Ceramic restoration with CAD-CAM ceramic coreGlass ceramic blocksFeldspathic porcelain blocks8- Ceramic restoration with copy milled ceramic core (Celay)Alumina blocks (Celay incerarn)MgAl,O, (Incerarn spinell)
39 PORCELAIN JACKET CROWN The all porcelain crown (PJC) has been around since a century. However, as mentioned before these were very brittle and fractured easily (halfmoon fractures). The marginal adaptation was also quite poor. Because of these problems its popularity gradually waned. This prompted McLean and Hughes to develop the PJC with an alumina reinforced core in This crown was developed in an attempt to improve the strength of the earlier porcelain jacket crowns. The increased content of alumina crystals (40 to 50 percent) in the core strengthened the porcelain by interruption of crack propagation
40 Types1- Porcelain jacket crown (traditional).2- Porcelain jacket crown with aluminous core.Note The above two are generally referred to as 'porcelain jacket crowns' or PJCs. The subsequently introduced ceramics are referred to as 'ceramic jacket crowns' or CJCs and 'glass ceramic crowns'.Technical ConsiderationsThe porcelain jacket crowns are made using the platinum foil matrix technique.Platinum Foil MatrixThe porcelain jacket crowns are constructed with high fusing feldspathic porcelains. A platinum foil is first adapted to the die. The platinum foil functions as matrix. It supports the porcelain during condensation and firing. After completion of the restoration the platinum foil matrix is discarded.Condensation and FiringThe platinum foil matrix is carefully removed from the die and the core porcelain is carefully condensed on to it. It is then placed in the furnace and fired. After cooling, the rest of the body is built up using dentin, enamel and other porcelainsRemoving the Foil After completion of the restoration the platinum foil is gently teased out and discarded. This can be quite difficult.
41 LEUCITE REINFORCED PORCELAIN (OPTEC HSP) Optec HSP is a feldspathic porcelain with a higher leucite crystal content (leucite reinforced). Its manipulation, condensation and firing is quite similar to the alumina reinforced porcelain jacket crowns (using platinum foil matrix).Advantages1- They are more esthetic because the core is less opaque (more translucent) when compared to the aluminous porcelain.2- Higher strength.3- No need of special laboratory equipment.Disadvantages1-Fit is not as good as metal ceramic crowns.2- Potential marginal inaccuracy.3- Not strong enough for posterior use.UsesInlays, onlays, veneers and low stress crowns.
42 CASTABLE GLASS CERAMIC (DICOR) The castable glass ceramic is quite unlike the previously mentioned porcelains. Its properties are more closer to that of glass and its construction is quite different. This is the only porcelain crown made by a centrifugal casting technique. The 'ceramming' process is also quite unique to this porcelain.
43 Fabrication of a Dicor Crown To understand the salient features of this material the step-by-step construction of a crown will be described:1- The crown pattern is first constructed in wax and then invested in investment material like a regular cast metal crown.2- After burning out the wax, nuggets of Dicor glass is melted and cast into the mould in a centrifugal casting machine.3- The glass casting is carefully recovered from the investment by sandblasting and the sprues are gently cut away.4- The glass restoration is then covered with a protective 'embedment material' '0 prepare it for the next stage called ceramming.5-Ceramming is a heat treatment process by which the glass is strengthened. Ceramming results in the development of microscopic crystals of mica, which improve the strength of the glass. It also reduces the transparency of the glass making it more opaque and less glass like.6-The cerammed glass is now built up with dentin and enamel (special veneering porcelain), condensed and fired to complete the restoration.
44 FeaturesThe Dicor glass-ceramic crown is very esthetic. This is because of the absence of an opaque core (unlike the previous porcelains). It also picks up some of the color from the adjacent teeth (chameleon effect) as well as from the underlying cement. Thus the color of the bonding cement plays an important role.UsesInlays, onlays, veneers and low stress crowns.
45 INJECTION MOULDED GLASS-CERAMIC (IPS EMPRESS ) This is another ceramic material which again is quite unlike the previous ceramics because of its unique way of fabrication (injection moulding). It is a precerammed glass-ceramic having a high concentration of leucite crystals. The manufacturer blends it with resins to form cylindrical blocks. The resins being thermoplastic, allows the material to be injection moulded.
46 Fabrication1- Using a wax pattern a mould is prepared in dental stone.2- The resin-ceramic block is heated to IS0aC and injected under air pressure of 1,500 psi into the mould.3- The core (or crown) is retrieved from the flask and fired for several hours to a maximum temperature of 1300°C. During the firing, the resin is burnt off leaving behind a rigid leucite reinforced ceramic core.4- The core is built up and fired using veneering porcelains in the conventional way.5- It can also be directly fabricated as a crown in which case, the crown is stained and glazed directly
47 Advantages1-The crown is supposed to be having a better fit (because of the lower firing shrinkage). 2-The esthetics is better because of the lack of metal or an opaque core. Disadvantages1-Need for costly equipment2- Potential of fracture in posterior areas.UsesInlays, onlays, veneers and low stress crowns.
48 GLASS INFILTRATED ALUMINA CORE (INCERAM) This ceramic system has a unique glass infiltration process and the first of its kind claimed for anterior bridge fabrication. The glass infiltration process compensated for firing shrinkage.Fabrication1- Two dies are required. One in stone and the other in refractory die material.2- A slurry of alumina is prepared and deposited on the refractory die using the slip cast method (the water from the slurry is absorbed by the porous die leaving a layer of alumina on the surface). The process is continued until a alumina coping of sufficient thickness is obtained.3-The fragile slip cast alumina coping is dried at 120cC for 2 hours.4-The alumina coping is sintered for 10 hours at 1100°C.5- The next step is glass infiltration. A slurry of glass material is applied on to the sintered alumina coping and fired for 3 to 5 hours at 1120°C. The glass fuses and infiltrates into the porous alumina coping.6- The excess glass forms a glassy layer on the surface which is trimmed off using special diamond burs.7- The coping is now ready for the rest of the build up using dentin and enamel veneering material
49 Advantages1- Good fit and marginal adaptation2- Good strength when compared to the earlier all ceramic crowns. Claimed to be strong enough for posterior single crowns and anterior bridge use.Disadvantages1-Comparatively less esthetic because of the opacity of the alumina core.2- Quite tedious to fabricate. Not all the bridges were successful, a few of them did fracture occasionally.UsesIn addition to the usual inlays, onlays, veneers and low stress crowns, this material can be used to construct low stress anterior bridges. Because of its occasional tendency to fracture when used for bridge construction its use should be carefully selected1-For people allergic to metal based bridges2- Where esthetics is absolutely critical
50 Glass Infiltrated Spinell Core (Inceram Spinell) Inceram spinell is an offshoot of In-ceram. Because ofthe comparatively high opacity of the alumina core, a new material was introduced known as Inceram spinell. It used MgAl204 instead of alumina. The fabrication is similar to the conventional Inceram. The Inceram spinell was more translucent and therefore more esthetic compared to the alumina core. Since the strength is lower, its use is limited to low stress situations.
51 CAD-CAM CERAMICSMany companies (e.g. Cerec, Germany) have come out with ceramics that can be ground into shape with the aid of a computer. These are known as computer aided design-computer aided machined ceramics or CAD-CAM ceramics.
52 Suppliedas Blocks of dense ceramic material, e.g. Feldspathic porcelain blocks (Vitablocs MK II) or glass-ceramic blocks (Dicor MGC).Fabrication1- The prepared crown or inlay cavity is scanned and fed into the computer.2- Signals from the computer operate the milling machine which grinds the internal surface of the inlay or crown in accordance with the scanned image. The earlier models ground only the internal surface. The external surface had to be manually ground. Current CAD-CAM machine models can grind the external surface also
53 Advantages1- Reduced chair time2- No need to make impression3- Reduced porosity, therefore greater strength4- Single appointment (especially for inlays). Disadvantages1- Costly equipment2- Scanning the preparation is technique sensitive.
54 COPY MILLED CERAMICSA new system (Celay by Mikron Technologies, Switzerland) uses a copy milling technique to produce ceramic cores or substructures for bridges. A similar copy milling process is used to produce duplicate keys. The original key is placed in the machine. A tool passes over the key tracing its outline. In the meantime, a milling machine simultaneously grinds a blank key to match the traced outline. The primary difference between this and the earlier system (CAD-CAM) is the manner in which the tooth dimensions are picked up. One scans the object whereas the other traces the object .
55 Blocks UsedCurrently blocks of Inceram and Inceram spinell are available for copy milling. Uses This technology is used to make substructures for crowns and bridges.Fabrication1-A pattern of the coping or substructure is created using a special blue2- The pattern may be created directly in the mouth or on a die made from an impression. The pattern is placed in the machine. A tracing tool passes over the pattern and guides a milling tool which grinds a copy of the pattern from a block of ceramic (Incerarn or In-ceram spinell). 3-The completed coping or bridge substructure is then glass infiltrated (as described earlier).4- The glass infiltrated substructure is built up with veneering porcelain and fired to complete the restoration.
56 PROPERTIES (GENERAL) OF FUSED PORCELAIN StrengthPorcelain has good strength. However, it is brittle and tends to fracture. The strength of porcelain is usually measured in terms of flexure strength (or modulus of rupture).Flexure strengthIt is a combination of compressive, tensile, as well as shear strength. Glazed porcelain is stronger than ground porcelain. (Ground MPa) (Glazed MPa).Compressive strength(331 MPa) Porcelain has good strength.Tensile strength(34 MPa) Tensile strength is low because of the unavoidable surface defects like porosities and microscopic cracks. When porcelain is placed under tension, stress concentrates around these imperfections and can result in brittle fractures.Shear strength (110 MPa) is low and is due to the lack of ductility caused by the complex structure of porcelain.Factors affecting strength- Composition- Surface integrity Surface imperfections like microscopic cracks and porosities reduce the strength.- Firing procedure Inadequate firing and overfiring weakens the structure.
57 Modulus of ElasticityPorcelain has high stiffness (69 GPa).Surface HardnessPorcelain is much harder (460 KHN) than natural teeth. It can wear natural teeth. Thus, it should be very carefully placed opposite natural teeth.Wear ResistanceThey are more resistant to wear than natural teeth.Thermal PropertiesThermal conductivity Porcelain has low thermal conductivity. Coefficient of thermal expansion (6.4 to 7.8 x lO-orC). It is close to that of natural teeth.Specific Gravity The true specific gravity of porcelain is The specific gravity of fired porcelain is usually less (2.2 to 2.3), because of the presence of air voids.Dimensional StabilityFired porcelain is dimensionally stable.
58 Chemical StabilityIt is insoluble and impermeable to oral fluids. Also it is resistant to most solvents. However, hydrofluoric acid causes etching of the porcelain surface. [A source of this is APF (acidulated phosphate fluoride) and stannous fluoride which are used as topical fluorides]. Hydrofluoric acid is used to etch the porcelain . Etching improves the bonding of the resin cement.
59 Esthetic PropertiesThe esthetic qualities of porcelain are excellent. It is able to match adjacent tooth structure in translucence, color and intensity (In addition, attempts have also been made to match the fluorescent property of natural teeth when placed under ultraviolet light, e.g. in discotheques). The color stability is also excellent. It can retain its color and gloss for years. Certain esthetic concerns have been raised when the dense opaquer layer is visible through thin crowns (in metal ceramic and Inceram crowns). However, this is more of an error in technique. The dentist must ensure an adequate depth of preparation (atleast 1.2 to 1.4 mm) to ensure sufficient thickness of dentin/enamel veneer to mask the opaquer. The technician on the other should ensure correct thickness of opaquer.
60 BiocompatibilityExcellent compatibility with oral tissues. CEMENTING OF CERAMIC RESTORATIONSThe type of cement used depends on the type of restoration (metal ceramic or full ceramic) and its location (anterior or posterior).Cementing All Ceramic Crowns, Inlays and VeneersBecause of the translucency of some all ceramic restorations (e.g. glass ceramic crowns), the underlying cement may influence the esthetics (color) of the restoration. Therefore the shade of the cement used should be carefully selected. Conventional cements may be used especially for most other crowns and bridges. However, veneers and inlays are best bonded with resin cements using the traditional acid etch technique. Resin bonding generates the high bond strengths needed for such restorations to succeed. Esthetics at the margins is certainly better with resin cements. Bonding of the cement to the porcelain can be improved by: Sandblasting ,Chemical etching. Sandblasting The inner surface of the ceramic restoration creates minute irregularities helping the cement to retain better. However, chemical etching appears to be superior.
61 Etching of PorcelainCertain ceramic restorations, especially veneers and inlays, have to be etched prior to bonding using resin cement. Etching improves the bond of the resin to the ceramic. Etching is done using hydrofluoric acid which attacks and selectively dissolves the inner surface of the ceramic. The tooth surface is also etched using phosphoric acid. Before placing the cement, a bond agent is applied to both surfaces (tooth and porcelain). Caution Extreme care must be taken when handling hydrofluoric acid. Severe acidic burns may result if it accidentally contacts the skin.Cementing Metal-Ceramic Crowns and BridgesThese are cemented like conventional restorations. The cement does not affect the esthetics because it is not visible through the restoration. Any convenient cement may be used.
62 PORCELAIN DENTURE TEETH Porcelain denture teeth are more natural looking than acrylic teeth. They have excellent biocompatibility and are more resistant to wear. Porcelain denture teeth also have the advantage of being the only type of denture teeth that allow the denture to be rebased. Porcelain teeth are made with high fusing porcelains. Two or more porcelains of different translucencies for each tooth are packed into metal moulds and fired on large trays in high temperature ovens. The retention of porcelain teeth on the denture base is by mechanical interlocking. Anterior teeth have projecting metal pins that get embedded in the denture base resin during processing. Posterior teeth on the other hand are designed with holes (diatoric spaces) in the underside into which the denture resin flows.
63 The disadvantages of porcelain denture teeth are: 1- They are brittle and make a clicking sound during contact.2- They require a greater interridge distance as they cannot be ground as thin as acrylic teeth in the ridge-lap areas without destroying the diatoric channels that provide their only means of retention.3- The higher density increases their weight.